Indentation hardness test, performed with either 3 gf or 9 gf loads, preceded the development of microhardness testers using traditional indenters. In 1925, Smith and Sandland of the UK developed an indentation test that employed a square-based pyramidal indenter made from diamond. They chose the pyramidal shape with an angle of 136° between opposite faces in order to obtain hardness numbers that would be as close as possible to Brinell hardness numbers for the specimen. The Vickers test has a great advantage of using one hardness scale to test all materials.The first reference to the Vickers indenter with low loads was made
Leeb rebound hardness test resulting in a greater value 1000×"v/v". A magnetic impact body permits the velocity to be deduced from the voltage induced by the body as it moves through the measuring coil. The quotient 1000×v/v is quoted in the Leeb rebound hardness unit HL. While in the traditional static tests the test force is applied uniformly with increasing magnitude, dynamic testing methods apply an instantaneous load. A test takes a mere 2 seconds and, using the standard probe D, leaves an indentation of just ~0.5 mm in diameter on steel or steel casting with a Leeb hardness of 600 HLD. By comparison,